# Expressing Crystallographic Textures through the Orientation Distribution Function: Conversion between Generalized Spherical Harmonic and Hyperspherical Harmonic Expansions

- 937 Downloads
- 6 Citations

## Abstract

In the analysis of crystallographic texture, the orientation distribution function (ODF) of the grains is generally expressed as a linear combination of the generalized spherical harmonics. Recently, an alternative expansion of the ODF, as a linear combination of the hyperspherical harmonics, has been proposed, with the advantage that this is a function of the angles that directly describe the axis and angle of each grain rotation, rather than of the Euler angles. This article provides the formulas required to convert between the generalized spherical harmonics and the hyperspherical harmonics, and between the coefficients appearing in their respective expansions of the ODF. A short discussion of the phase conventions surrounding these expansions is also presented.

## 1 Introduction

*ϕ*

_{1}, Φ, and ϕ

_{2}, and the consequent series expansion of the ODF as a linear combination of generalized spherical harmonics

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) in the form

^{1}of rotations.[18] A quaternion, in this context, is a normalized four-vector with components given by

*ω*is the angle of rotation and

*θ*and

*ϕ*are the polar and azimuthal angles of the rotation axis, respectively. The rotation corresponding to a quaternion is readily apparent from the final three components, which form a vector that points along the axis of rotation and scales monotonically in length with the rotation angle.[19] This close relationship of a quaternion with the axis and angle of a rotation further permits the construction of an orientation space that is substantially simpler to visualize and interpret than that of the Euler-angle parameterization.[20] With regard to the manipulation of the orientation information, the most familiar example of the advantage of quaternions is given by the formula for the multiplication of rotations, which involves only a bilinear combination of the quaternion components.[21] Other instances in which the use of quaternions simplifies calculations related to the analysis of orientation information appear throughout the literature.[11,15,22,23]

*S*

^{3}(the unit sphere in four-dimensional space). Analogous to the expansion of a square-integrable function on

*S*

^{2}(the unit sphere in three-dimensional space) as an infinite linear combination of the spherical harmonics, a square-integrable function on

*S*

^{3}may be expanded as an infinite linear combination of the hyperspherical harmonics

*Z*

_{l,m}

^{n}(

*ω*,

*θ*,

*ϕ*), or

*n*is restricted to even integers by the trivial symmetry of three-dimensional space. This expansion is discussed in more detail elsewhere.[20]

Because the physical significance of orientation information does not depend on the means by which it is described, the expansions given in Eqs. [1] and [4] may in principle be used interchangeably. However, there is presently no means of converting an ODF expressed in the form of the generalized spherical harmonic expansion of Eq. [1] to one in the form of the hyperspherical harmonic expansion of Eq. [4]. With this in mind, the purpose of this article is principally to provide continuity with the existing literature by deriving a simple linear transformation to relate the coefficients of these two expansions. Our expectation is that this will allow extant published results in texture analysis formulated by means of the traditional series expansion to be converted to, and presented in, a more intuitive and readily accessible form. This result is then harnessed to apply a mathematical technique in common use with the generalized spherical harmonic expansion to the hyperspherical harmonic expansion.

## 2 Problem Formulation

The group of primary concern to the study of crystallographic orientations is *SO*(3), the group of rotations of three-dimensional space. While the importance of this group to the physical sciences has encouraged many authors to investigate its properties, the resulting treatments do not always follow a consistent set of conventions.[12,18,24,25] At least for the current authors, this situation has caused a certain degree of confusion and inconvenience, as the conventions used in deriving many of the results available in the literature are not always explicitly stated. To our knowledge, the results contained in this article do not appear anywhere else in the literature with a consistent set of conventions.

We follow the same conventions in the interpretation and use of a rotation matrix as does Altmann.[18] That is, a rotation operation is viewed as an active rotation of configuration space rather than as a passive rotation of the coordinate system, unless explicitly stated otherwise. A rotation matrix left-multiplies the column vector of the coordinates of a point, and right-multiplies the row vector of the components of a basis. This interpretation allows one to identify a crystal orientation with the rotation operation required to bring a reference crystal into coincidence with the actual crystal. The ODF is then interpreted as a function of rotations of three-dimensional space or, more often, as a function of some set of parameters that clearly define a rotation.

This article makes use of two parameterizations. The first of these is the Euler angles *ϕ*_{1}, Φ, and *ϕ*_{2}, which define a general rotation as the result of three consecutive active rotations by the angles −*ϕ*_{1}, −Φ, and −*ϕ*_{2} about the *z*, *x*, and *z* axes, respectively (from the point of view of an observer attached to the coordinate system, this active rotation sequence is identical to the passive rotation sequence defining the Euler angles as described by Bunge[10]). The second rotation parameterization is by the axis-angle parameters *ω*, *θ*, and *ϕ*, as described earlier. The relationship of the Euler angles to the axis-angle parameters is visible from the explicit conversion formulas provided in Appendix A.

The analytical form of the ODF used by the majority of the crystallography community is provided in Eq. [1], in which rotations are parameterized as sets of Euler angles. This equation actually derives from one of the consequences of the Peter–Weyl theorem, namely that the matrix elements of the irreducible representations of *SO*(3) provide a complete, orthogonal basis for the expansion of a square-integrable function of three-dimensional rotations.[26] While many equivalent expressions for the irreducible representations of *SO*(3) appear in the literature, they often differ from one another by similarity transformations.[12,18,24,25] Once a set of conventions is specified and a consistent expression is found, the Peter–Weyl theorem allows the ODF to be written as an infinite linear combination of the matrix elements of these irreducible representations. For example, the expansion in Eq. [1] is found by following the phase convention of Bunge,[10] expressing the matrix elements of the irreducible representations of *SO*(3) as functions of the Euler angles, and denoting the matrix element in row *m*′ and column *m* of the (2*l*+1)-dimensional irreducible representation by *T*_{l}^{m′,m}(*ϕ*_{1}, Φ, *ϕ*_{2}).

The expansion provided in Eq. [4] follows more directly from a consideration of *SO*(4), the group of rotations of four-dimensional space, than from *SO*(3). A well-known result of group theory states that the basis elements of the irreducible representations of a group of operators provide a complete, orthogonal basis for the expansion of a function to which an operation of the group may be applied.[24] Because sets of the hyperspherical harmonics *Z*_{l,m}^{n}(*ω*, *θ*, *ϕ*) transform as the bases of the irreducible representations of *SO*(4), the hyperspherical harmonics form a complete, orthogonal basis for the expansion of a square-integrable function on *S*^{3}. Considering points on *S*^{3} to correspond to normalized quaternions, Eq. [3] suggests that the axis-angle parameters identify points on *S*^{3} in a manner analogous to that of the spherical angles on *S*^{2}. That is, exactly as a function on *S*^{2} is more naturally written as a function of the spherical angles than of Cartesian coordinates, a function on *S*^{3} is more naturally written as a function of the axis-angle parameters than of quaternion coordinates. The axis-angle parameterization is therefore entirely compatible with the interpretation of the ODF as a square-integrable function on *S*^{3}, which allows the ODF to be written as an infinite linear combination of the hyperspherical harmonics in Eq. [4].

Regardless of the different motivations for the generalized spherical harmonic and the hyperspherical harmonic expansions, they contain the same orientation information. As such, there must be a method to convert from one expansion to the other. This expansion is found by comparing the expressions for the matrix elements of the irreducible representations of *SO*(3) in the Euler-angle and axis-angle parameterizations. When written using the Euler angles, the expression for these matrix elements gives the formula for the generalized spherical harmonics. When written using the axis-angle parameters, the same expression becomes a linear combination of the hyperspherical harmonics. Equating these forms gives the conversion of the basis functions in Eq. [1] to the basis function in Eq. [4], and the conversion from the coefficients in Eq. [1] to the coefficients in Eq. [4] as well. We develop this approach further in Sections III to V.

## 3 Rotation Conventions and the Generalized Spherical Harmonics

There are many mathematical results in the literature that are useful and relevant for the present problem. However, incorporating or referring to them without establishing a consistent set of conventions is quite hazardous. In particular, the conversion from the generalized spherical harmonics to the hyperspherical harmonics is nonsensical unless a consistent set of conventions is used to derive the expressions for the matrix elements of the irreducible representations of *SO*(3) as functions of the Euler-angle and axis-angle parameters. We therefore devote a significant portion of this article to the consideration of this issue.

*P*

_{l}

^{m′,m}(cos Φ) is defined as

*m*′ and column

*m*of the (2

*l*+1)-dimensional irreducible representation of

*SO*(3). Therefore, Eq. [6] depends implicitly on the conventions adopted by Bunge[10] during the construction of the irreducible representations. Generally speaking, the range of conventions that must be specified include the selection of the basis elements, the choice of the active or passive rotation convention, and the parameterization used to write the formulas for the resulting matrix elements.

The vast majority of literature on the subject, including that by Bunge[10] and the current article, selects the set of spherical harmonics with a particular value of *l* as the basis elements of the (2*l*+1)-dimensional irreducible representation of *SO*(3). Because the basis is consistent throughout, the issue is not discussed further. As for the remaining conventions enumerated earlier, Bunge[10] uses the passive convention and the Euler-angle parameterization, while the current article uses the active convention and the axis-angle parameterization. The comparison of matrix elements apparently requires that the relationship of the representations constructed following these different conventions be clearly established. We address these differences individually for the sake of clarity, with the difference in rotation convention first and the difference in parameterization second.

Regarding the difference in rotation convention, consider that the elements of a rotation matrix depend only on the selection of an initial coordinate system and the apparent rotation of space from the perspective of an observer rigidly attached to that coordinate system. If two matrices that effect the same apparent transformation of space share a single basis, then corresponding matrix elements of the two matrices should be the same, independent of the rotation convention followed. In particular, sequential active rotations by −*ϕ*_{1} about the *z*-axis, −Φ about the *x*-axis, and −*ϕ*_{2} about the *z*-axis effect the same apparent transformation of space as sequential passive rotations by *ϕ*_{1} about the *z*-axis, by *Φ* about the *x*′-axis, and by *ϕ*_{2} about the *z*″-axis. Therefore, the elements of the matrix describing the active rotation sequence should be the same as the elements of the matrix describing the passive rotation sequence.

Define the function *D*_{m′,m}^{l}(*ϕ*_{1}, Φ, *ϕ*_{2}) as the matrix element in row *m*′ and column *m* of the (2*l*+1)-dimensional irreducible representation of *SO*(3), in which the representation is considered to describe the active rotation sequence referred to earlier, *i.e*., to follow the active convention. The explicit formula for this function is derived in Appendix B. Because the generalized spherical harmonic *T*_{l}^{m′,m}(*ϕ*_{1}, Φ, *ϕ*_{2}) apparently differs only in that the corresponding representation is considered to describe the passive rotation sequence referred to earlier, these functions should be identical, *i.e*., *T*_{l}^{m′,m}(*ϕ*_{1}, Φ, *ϕ*_{2}) = *D*_{m′,m}^{l}(*ϕ*_{1}, Φ, *ϕ*_{2}).

*SO*(3) by

*T*

_{m′,m}

^{l}(

*ϕ*

_{1},

*θ*,

*ϕ*

_{2}),[27]

*t*

_{m′,m}

^{l}(

*ϕ*,

*θ*,

*ψ*),[12] and

**D**^{(l)}({

*α*,

*β*,

*γ*})

_{m′,m},[24] respectively. Inserting

*ϕ*

_{1}, Φ, and

*ϕ*

_{2}for the angles of the first, second, and third rotations, respectively, of these functions, we find that their relationships to the generalized spherical harmonics

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) are

*ϕ*

_{1}, Φ, and

*ϕ*

_{2}for the angles of the first, second, and third rotations, respectively, of these functions does not adequately address the conventions concerning the use of these functions. We therefore find that the question of consistency of conventions pervades the literature and that it is quite difficult to resolve the difference between

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) and

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) in Eq. [8] without clearly establishing the source of the generalized spherical harmonics.

Regardless of the conventions followed in deriving the traditional form of the generalized spherical harmonics, the expansion in Eq. [1] remains a valid expansion of the ODF; changing the generalized spherical harmonics by a constant factor amounts to pulling a constant factor out of the coefficients in the expansion. Because Bunge used the generalized spherical harmonics almost exclusively in the context of Eq. [1], the question of the constant factor appearing in Eq. [8] is virtually irrelevant to his subsequent results. For the purposes of the present article, however, a constant factor represents a change in the values of the matrix elements of the irreducible representations of *SO*(3). Equating expressions for the matrix elements in different parameterizations certainly gives nonsensical results when the expressions are not equal. Within this article, the functions *D*_{m′,m}^{l}(*ϕ*_{1}, Φ, *ϕ*_{2}) will therefore be considered as more fundamental from the standpoint of calculations, although the majority of our equations will be formulated using the functions *T*_{l}^{m′,m}(*ϕ*_{1}, Φ, *ϕ*_{2}) in order to relate our results more directly to the literature.

## 4 Rotation Conventions and Hyspherical Harmonics

*n*, 0 ≤

*l*≤

*n*, and −

*l*≤

*m*≤

*l*. The

*C*

_{n−l}

^{l+1}is a Gegenbauer polynomial and

*P*

_{l}

^{m}is an associated Legendre function.[32,33] Complex conjugation of Eq. [10] reveals one of the properties of the hyperspherical harmonics to be

*m*′ and column

*m*of the (2

*l*+1)-dimensional irreducible representation of

*SO*(3) may be written as a linear combination of the hyperspherical harmonics[34,35]

*C*

_{l,m′,λ,μ}

^{l,m}is a Clebsch–Gordan coefficient, as defined in Appendix C, and vanishes unless the summation indices satisfy the conditions 0 ≤

*λ*≤ 2

*l*and

*μ*=

*m*−

*m*′. The irreducible representation corresponding to

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*) is considered to describe an active rotation in the axis-angle parameterization.

The arrangement of indices on the hyperspherical harmonics as used here differs from that of Reference 20, in consideration that the index *n* identifies the set of hyperspherical harmonics that form a basis for the (*n*+1)^{2}-dimensional irreducible representation of *SO*(4), while the indices *l* and *m* identify a single member of this set. The difference in the significance of these indices encourages that they be separated accordingly. The phase of the hyperspherical harmonic differs from that of our previous work as well;[20] some motivation for this departure will be given presently.

### 4.1 Phase of Hyperspherical Harmonics

A reasonable condition that the phase of the hyperspherical harmonics defined in Eq. [10] must satisfy is revealed by investigating the properties of *SO*(3). While not necessarily obvious, the irreducible representations of *SO*(3) as presented in the literature are entirely compatible with the canonical representation of three-dimensional rotations as three-by-three real orthogonal matrices of the determinant one. That is, there exists a similarity transformation that brings the three-by-three irreducible representation of *SO*(3) into the familiar canonical form. Furthermore, the linear transformation effecting this similarity transformation, when right-multiplying the row vector of the basis elements of the three-by-three irreducible representation, brings the basis into a form that behaves identically to the usual unit vectors of three-dimensional space. Although requiring that this similarity transformation exist places a certain constraint on the relationship of the irreducible representation to the basis elements, the ability to freely select the similarity transformation permits an infinite number of equivalent forms for the irreducible representations and the basis elements. The Condon–Shortley phase convention uniquely determines a standard similarity transformation, however, and allows the irreducible representations of *SO*(3) to be given in a consistent form throughout the literature.

The situation is rather different with irreducible representations of *SO*(4) and the hyperspherical harmonics. There does not appear to be any counterpart to the Condon–Shortley phase convention to uniquely specify the form of the irreducible representations of *SO*(4) and the phase of the hyperspherical harmonics, as is reflected in the variety of phases for the hyperspherical harmonics appearing in the literature.[28, 29, 30, 31] Nevertheless, the requirement that the four-by-four irreducible representation of *SO*(4) and the four hyperspherical harmonics for which *n* = 1 be related in the manner described earlier is certainly reasonable. That is, we require that there exist an invertible linear transformation of the hyperspherical harmonics that makes the resulting basis behave identically to the orthogonal unit vectors along the *w*, *x*, *y*, and *z* axes of four-dimensional space and that simultaneously defines a similarity transformation of the four-by-four irreducible representation that brings the representation into the canonical form.

*SO*(4), which is, generally speaking, not as familiar as for

*SO*(3). We consider the canonical form for these representations as deriving from the multiplication rule for normalized quaternions. Given a rotation represented by the quaternion

*q*that is followed by a rotation represented by the quaternion

*g*, there exists a single equivalent rotation represented by the quaternion

*u*. One of the particularly convenient properties of the quaternion parameterization is that this multiplication rule is bilinear,[11] which means that there is a four-by-four real orthogonal matrix of determinant one,

*G,*that, when left-multiplying the column vector of the components of the quaternion

*q*, returns the column vector of the components of the quaternion

*u,*or[21]

*q*that is preceded by a rotation represented by the quaternion

*h*, there exists a single equivalent rotation represented by the quaternion

*v*. There is then a four-by-four real orthogonal matrix of determinant one,

*H*, that, when left-multiplying the column vector of the components of the quaternion

*q*, returns the components of the quaternion

*v*, or[21]

*G*and

*H*separately perform distinct, constrained four-dimensional rotations, the matrix formed by their product is a general four-by-four real orthogonal matrix of the determinant one and performs a general four-dimensional rotation. Because

*G*and

*H*commute, the order of application of these matrices does not change the result. This provides a canonical form for four-dimensional rotations.

*SO*(4) by a similarity transformation of the direct product of irreducible representations of

*SO*(3), that is,[20,34]

*λ*′ and in decreasing values of

*μ*′ for a particular

*λ*′, and with columns ordered similarly, by

*R*. The basis of this representation is formed by the four hyperspherical harmonics for which

*n*= 1. We require then that there exists an invertible linear transformation

*B*of the hyperspherical harmonics that defines functions that behave analogously to the unit vectors along the

*w*,

*x*,

*y*, and

*z*axes, and that

*B*simultaneously defines a similarity transformation that brings the matrix

*R*into the canonical form. A suitable linear transformation exists, and is defined by the relation

*w*,

*x*,

*y*, and

*z*, respectively. The matrix

*B*

^{−1}

*RB*is equivalent to

*G*when

*ω*

_{2}= 0, and to

*H*when

*ω*

_{1}= 0, that is, this similarity transformation brings the irreducible representation into canonical form.

While these developments are not intended as a rigorous justification for the choice of phases for the hyperspherical harmonics, the hyperspherical harmonics defined in Eq. [10] and the irreducible representations of *SO*(4) defined in Eq. [15] appear to be reasonable inasmuch as they satisfy the compatibility condition outlined earlier.

### 4.2 Relationship of Basis Functions

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) and

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) established by Eq. [8], there remains the question of the relationship of

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) and

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*). For this, an inspection of the rotation operations corresponding to

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}),

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) and

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*) is useful. According to Bunge,[10]

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) identifies a crystal orientation with the passive rotation that brings the sample coordinate system into coincidence with the crystal coordinate system, in which the crystal is in the actual orientation throughout. This operation is shown at the top of Figure 1. As discussed in Section III,

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) identifies a crystal orientation with the active counterpart to

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}),

*i.e*., with the active rotation that brings the crystal from the actual orientation into coincidence with the reference orientation, in which the coordinate system is aligned with the sample throughout. This operation is shown in the middle of Figure 1. By definition,[34]

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*) identifies a crystal orientation with the active rotation that brings the crystal from the reference orientation into coincidence with the actual orientation, in which the coordinate system is aligned with the sample throughout. This operation is shown at the bottom of Figure 1.

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) is the inverse of the active rotation corresponding to

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*). That is, the unitary matrix constructed from

*D*

_{m′,m}

^{l}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}) is the inverse of the unitary matrix constructed from

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*), or

*T*

_{l}

^{m′,m}(

*ϕ*

_{1}, Φ,

*ϕ*

_{2}), formulated with the passive convention and the Euler-angle parameterization, to

*U*

_{m′,m}

^{l}(

*ω*,

*θ*,

*ϕ*), formulated with the active convention and the axis-angle parameterization, and is the basis for the conversion formulas presented in Section V.

## 5 Conversion Formulas

*SO*(3) must be independent of the parameterization, the formulas for these matrix elements in the Euler-angle and axis-angle parameterizations may be equated. Inverting Eq. [18] and inserting Eq. [12] indicates that

*m*and

*m*′, complex-conjugating both sides and applying Eq. [11], this becomes

*μ*to a summation over −

*μ*and applying the symmetry properties of the Clebsch–Gordan coefficients gives the result

*C*

_{l,−m′,l,m}

^{λ′,μ′}, summing over the indices −

*m*′ and

*m*, and rearranging the summations then gives

*δ*

_{λ′,λ}

*δ*

_{μ′,μ}by the unitarity of the Clebsch–Gordan coefficients, simplifying the equation to

*m*′ with a summation over

*m*′ gives

*m*−

*m*′ =

*μ*. This is the counterpart to Eq. [21], and establishes the formula to convert from the hyperspherical harmonics to the generalized spherical harmonics.

*π*

^{2}everywhere. As with the matrix elements of the irreducible representations of

*SO*(3), equating expansions of the ODF when the values of the ODFs at corresponding points are not equal is nonsensical. This disparity is resolved by multiplying one of the expansions by the appropriate coefficient, or

*vice*

*versa*; the required Clebsch–Gordan coefficients are given in Appendix C.

## 6 Example

*z*

_{l,m}

^{n}of the hyperspherical harmonic expansion as calculated directly from fitting the experimental data with Eq. [5], and as calculated by first fitting for the coefficients

*t*

_{l}

^{m′,m}of the generalized spherical harmonic expansion from Eq. [2] and then converting them to the

*z*

_{l,m}

^{n}by means of Eq. [29]. The analytical expression for an ODF should be independent of the calculation method, so the equivalence of these sets of coefficients provides evidence for the accuracy of the formulas derived in the Section V.

*n*≤ 30, and the procedure used to display the hyperspherical harmonic expansions graphically is described elsewhere.[20] Blue and red regions correspond to positive and negative probability density, respectively. The presence of a few clearly distinguishable probability density peaks reflects that the observed region contained only a few grains, while the resemblance of Figure 3(a) to Figure 3(b) indicates that the directly calculated coefficients match well with those calculated by means of the conversion formulas. Although not practical to present in print, we have directly compared the numerical values of the 5456 coefficients in the two expansions as well, and they are equal to within one part per 10

^{8},

*i.e*., to within the error of the numerical calculations. These results convincingly validate the mathematical conclusions in the Section V.

## 7 Positivity Constraint

We anticipate that the conversion formulas presented in Section V will allow existing texture information to be translated easily into the new hyperspherical harmonic-based representation. Beyond texture information, however, the conversion formulas carry the broader implication that mathematical methods and tools developed for use with the generalized spherical harmonics do not need to be rederived for the hyperspherical harmonics. One example is provided by the positivity method for the correction of the ghost error, which was handled in the context of the generalized spherical harmonic expansion by prior researchers.[36, 37, 38]

The regions of negative probability density appearing in Figure 3 are unphysical, and result from the truncation of the infinite expansion to a finite number of terms. Historically speaking, regions of negative probability density often appeared in the generalized spherical harmonic expansion of the ODF, although this phenomenon was generally attributed to the inherent limitations on the information obtained from conventional diffraction experiments (*i.e*., the so-called “ghost error”) rather than truncation error. Many of the same techniques developed in the literature to correct for the ghost error may be used to correct for the truncation error as well. Roughly, these include the positivity method,[36, 37, 38] the quadratic method,[39,40] and the maximum entropy method.[41, 42, 43, 44] Of these, the positivity method is arguably the simplest to implement. This traditionally involves finding an approximation for the odd *l* coefficients in Eq. [1] by enforcing the non-negativity of the ODF.

*f*

_{0}(

*g*) that is calculated using only the even

*l*coefficients, define a function

*l*coefficients of

*f*

_{0}(

*g*) and the odd

*l*coefficients of \( \hat{f}_{1} \left( g \right) \) to define the function

*f*

_{1}(

*g*). From this point on, the positivity method follows an iterative procedure. Insert

*f*

_{i}(

*g*) into Eq. [30] to define a function \( \hat{f}_{i+1} \left( g \right) \), and find the expansion coefficients of this function from Eq. [2]. Define the function

*f*

_{i+1}(

*g*) from the even

*l*coefficients of

*f*

_{i}(

*g*) and the sum of the odd

*l*coefficients of \( \hat{f}_{i+1} \left( g \right) \) and

*f*

_{i}(

*g*), and repeat the procedure until the magnitude of the negative probability density in

*f*

_{i+1}(

*g*) falls below a set threshold. The function

*f*

_{i+1}(

*g*) is called the complete ODF.

The same general principle, with minor modifications, may be used to reduce the extent of the truncation error in Figure 3. Indicate the hyperspherical harmonic expansion of the ODF by *f*_{0}(*g*). Insert this function into Eq. [30] to find \( \hat{f}_{1} \left( g \right) \), and calculate the expansion coefficients of \( \hat{f}_{1} \left( g \right) \) from Eq. [5]. Form the sum of every coefficient of *f*_{0}(*g*) with the corresponding coefficient of \( \hat{f}_{1} \left( g \right) \), and normalize the result by multiplying each coefficient by the constant that brings *z*_{0,0}^{0} to the value \( {1 \mathord{\left/ {\vphantom {1 {\sqrt 2 \pi }}} \right. \kern-\nulldelimiterspace} {\sqrt 2 \pi }} \). This collection of coefficients defines the function *f*_{1}(*g*), which is a normalized approximation to \( f_{0} \left( g \right) + \hat{f}_{1} \left( g \right) \). This procedure is iteratively repeated, using Eq. [30] to find \( \hat{f}_{i+1} \left( g \right) \) from *f*_{i}(*g*), until the magnitude of the negative probability density in *f*_{i+1}(*g*) falls below a set threshold. (The difference between this method and the positivity method outlined earlier is the fact that EBSD measurements provide information about all the coefficients in the expansion; this removes the need to preserve the values of some coefficients while selectively changing others.)

## 8 Conclusions

While the importance of the generalized spherical harmonic expansion of an ODF to the historical development of texture analysis is undeniable, exclusive reliance on a single series expansion is inherently limiting. This is quite clear from an examination of the literature, in which discrete orientations are routinely manipulated with multiple parameterizations (rotation matrices, Rodrigues vectors, Euler angles, *etc*.) to leverage their complementary strengths, but series expansions of orientation distributions in the past were restricted to this single representation. The absence of an alternative to the generalized spherical harmonic expansion essentially required that every operation on the ODF be performed in the Euler-angle parameterization, regardless of its suitability. The hyperspherical harmonic expansion of an ODF provides the missing alternative, although the utility of this series expansion relies on the existence of a means by which to efficiently and easily convert from one representation to the other; this article provides the equations effecting this conversion for the first time.

The ramifications of these conversion formulas are expected to extend further than the ability to express a particular ODF by a series expansion in the axis-angle parameterization. Specifically, these formulas provide continuity of the hyperspherical harmonic expansion with the existing literature and allow mathematical results derived using the generalized spherical harmonic expansion (or programs written using this expansion) to be used with a minimum of modification. As a simple example, the fact that the conversion of the expansion coefficients is a linear transformation enables one of the procedures existing in the literature to enforce a positivity condition on the generalized spherical harmonic expansion of the ODF to be applied directly to the hyperspherical harmonic expansion of the ODF. We hope that these results significantly increase the accessibility and utility of the hyperspherical harmonic expansion in the field of texture analysis.

## Footnotes

- 1.
Throughout the remainder of this article, the reader should understand all quaternions to be normalized,

*i.e*., of unit length.

## Notes

### Acknowledgments

This work was supported by the United States National Science Foundation under Contracts DMR‐0346848 and DMR‐0855402.

### References

- 1.F. Emren, U. Vonschlippenbach, and K. Lucke:
*Acta Metall*., 1986, vol. 34, pp. 2105–17.CrossRefGoogle Scholar - 2.J.B. Clark, R.K. Garrett, T.L. Jungling, R.A. Vandermeer, and C.L. Vold:
*Metall. Trans. A*, 1991, vol. 22, pp. 2039–48.CrossRefGoogle Scholar - 3.E. Nakamachi, C.L. Xie, H. Morimoto, K. Morita, and N. Yokoyama:
*Int. J. Plast.*, 2002, vol. 18, pp. 617–32.MATHCrossRefGoogle Scholar - 4.G. Proust and S.R. Kalidindi:
*J. Mech. Phys. Solids*, 2006, vol. 54, pp. 1744–62.MATHCrossRefMathSciNetADSGoogle Scholar - 5.J.V. Bernier, M.P. Miller, and D.E. Boyce:
*J. Appl. Crystallogr*., 2006, vol. 39, pp. 697–713.CrossRefGoogle Scholar - 6.T. Bohlke, U.U. Haus, and V. Schulze:
*Acta Mater.*, 2006, vol. 54, pp. 1359–68.CrossRefGoogle Scholar - 7.R. Hielscher and H. Schaeben:
*J. Appl. Crystallogr.*, 2008, vol. 41, pp. 1024–37.CrossRefGoogle Scholar - 8.H.J. Bunge:
*Mber. Dt. Akad. Wiss.*, 1965, vol. 7, pp. 351–60.MATHMathSciNetGoogle Scholar - 9.R.-J. Roe:
*J. Appl. Phys*., 1965, vol. 36, pp. 2024–31.CrossRefADSGoogle Scholar - 10.H.J. Bunge:
*Texture Analysis in Materials Science: Mathematical Methods*, Cuvillier Verlag, Gottingen, Germany, 1993, pp. 4–8, 47–52, 351–56.Google Scholar - 11.J. Stuelpnagel:
*SIAM Rev.*, 1964, vol. 6, pp. 422–30.MATHCrossRefMathSciNetGoogle Scholar - 12.N.J. Vilenkin:
*Special Functions and the Theory of Group Representations*, American Mathematical Society, Providence, RI, 1968, pp. 97–146.MATHGoogle Scholar - 13.M. Siemens, J. Hancock, and D. Siminovitch:
*Solid State Nucl. Mag*., 2007, vol. 31, pp. 35–54.CrossRefGoogle Scholar - 14.J.W. Zhao and B.L. Adams:
*Acta Crystallogr. A*, 1988, vol. 44, pp. 326–36.CrossRefGoogle Scholar - 15.H. Grimmer:
*Acta Crystallogr. A*, 1980, vol. 36, pp. 382–89.CrossRefMathSciNetADSGoogle Scholar - 16.A. Heinz and P. Neumann:
*Acta Crystallogr. A*, 1991, vol. 47, pp. 780–89.CrossRefMathSciNetGoogle Scholar - 17.A. Morawiec and D.P. Field:
*Philos. Mag. A*, 1996, vol. 73, pp. 1113–30.CrossRefADSGoogle Scholar - 18.S.L. Altmann:
*Rotations,**Quaternions, and Double Groups*, Clarendon Press, Oxford, United Kingdom, 1986, pp. 29–64, 201–24, 237–47.Google Scholar - 19.F.C. Frank:
*Metall. Trans. A*, 1988, vol. 19A, pp. 403–08.ADSGoogle Scholar - 20.J.K. Mason and C.A. Schuh:
*Acta Mater*., 2008, vol. 56, pp. 6141–55.CrossRefGoogle Scholar - 21.A. Hanson:
*Visualizing Quaternions*, Morgan Kaufmann, San Francisco, CA, 2005, pp. 433–38.Google Scholar - 22.A. Morawiec:
*J. Appl. Crystallogr.*, 1990, vol. 23, pp. 374–77.CrossRefGoogle Scholar - 23.M. Humbert, N. Gey, J. Muller, and C. Esling:
*J. Appl. Crystallogr.*,1996, vol. 29, pp. 662–66.CrossRefGoogle Scholar - 24.E.P. Wigner:
*Group Theory and Its Application to the Quantum Mechanics of Atomic Spectra*, Academic Press, New York, NY, 1959.MATHGoogle Scholar - 25.M.E. Rose:
*Elementary Theory of Angular Momentum*, Dover, New York, NY, 1995, pp. 48–75, 222–42.Google Scholar - 26.A.W. Knapp:
*Representation Theory of Semisimple Groups: An Overview Based on Examples*, Princeton University Press, Princeton, NJ, 1986, pp. 14–22.MATHGoogle Scholar - 27.I.M. Gel’fand, R.A. Minlos, and Z.Y. Shapiro:
*Representations of the Rotation and Lorentz Groups and Their Applications*, Pergamon Press (distributed in the Western Hemisphere by Macmillan), New York, NY, 1963.MATHGoogle Scholar - 28.M. Bander and C. Itzykson:
*Rev. Mod. Phys*., 1966, vol. 38, pp. 330–45.CrossRefMathSciNetADSGoogle Scholar - 29.L.C. Biedenharn:
*J. Math. Phys*, 1961, vol. 2, pp. 433–41.MATHCrossRefMathSciNetADSGoogle Scholar - 30.G. Domokos:
*Phys. Rev*., 1967, vol. 159, pp. 1387–1403.CrossRefADSGoogle Scholar - 31.A.V. Meremianin:
*J. Phys. A: Math. Gen.*, 2006, vol. 39, pp. 3099–3112.MATHCrossRefMathSciNetADSGoogle Scholar - 32.H. Bateman and A. Erdélyi:
*Higher Transcendental Functions*, McGraw-Hill, New York, NY, 1953.Google Scholar - 33.I.S. Gradshtein, I.M. Ryzhik, and A. Jeffrey:
*Table of Integrals, Series, and Products*, Academic Press, New York, NY, 1965, pp. 1014–16, 1025–31.Google Scholar - 34.J.K. Mason:
*Acta Cryst. A*, 2009, vol. 65, pp. 259–66.CrossRefGoogle Scholar - 35.D.A. Varshalovich, A.N. Moskalev, and V.K. Khersonskii:
*Bull. Acad. Sci. USSR Phys. Ser.*, 1974, vol. 38, pp. 1711–26.Google Scholar - 36.M. Dahms and H.J. Bunge:
*Text. Microstruct.*, 1988, vol. 10, pp. 21–35.CrossRefGoogle Scholar - 37.M. Dahms and H.J. Bunge:
*J. Appl. Crystallogr.*, 1989, vol. 22, pp. 439–47.CrossRefGoogle Scholar - 38.F. Wagner, M. Humbert, J. Muller, and C. Esling:
*Europhys. Lett*., 1990, vol. 11, pp. 479–83.CrossRefADSGoogle Scholar - 39.P. Vanhoutte:
*Text. Microstruct*., 1983, vol. 6, pp. 1–19.CrossRefGoogle Scholar - 40.P. Vanhoutte:
*Text. Microstruct*., 1991, vol. 13, pp. 199–212.CrossRefGoogle Scholar - 41.H. Schaeben:
*J. Appl. Phys*., 1988, vol. 64, pp. 2236–37.CrossRefADSGoogle Scholar - 42.F. Wang, J.Z. Xu, and Z.D. Liang:
*Text. Microstruct.*, 1989, vol. 10, pp. 217–26.CrossRefGoogle Scholar - 43.H. Schaeben:
*J. Appl. Phys*.,1991, vol. 69, pp. 1320–29.CrossRefADSGoogle Scholar - 44.F. Wang, J.Z. Xu, and Z.D. Liang:
*Text. Microstruct.*, 1992, vol. 19, pp. 55–58.CrossRefGoogle Scholar - 45.D.A. Varshalovich, A.N. Moskalev, and V.K. Khersonskii:
*Quantum Theory of Angular Momentum*, World Scientific, Singapore, 2008, pp. 235–89.Google Scholar - 46.G. Racah:
*Phys. Rev.*, 1942, vol. 62, pp. 438–62.CrossRefADSGoogle Scholar